(2) L. Monteagudo-Lerma et al. / Thin Solid Films 545 (2013) 149–153. formula . The surface roughness of the AlN layers was measured by atomic force microscopy (AFM) in the tapping mode with a Veeco Dimension 3100 microscope. Data visualization and processing were carried out using the WSxM software . 3. Results and discussion 3.1. Deposition of AlN layers under unbiased substrate conditions. 3.5. 1.2. 3.0. 0.8. 2.5. 0.4. 2.0. 0.0 100. 125. 150. 175. RF Power (W). The adequate tuning of the substrate bias during deposition can be a critical parameter to improve the crystalline quality of the AlN layers . In this section, we describe the effect of substrate bias on the structural quality and surface morphology of AlN layers, using the abovedetermined deposition conditions (sputtering pressure = 0.47 Pa in pure nitrogen atmosphere, PRF = 150 W and Tsubs = 450 °C). Considering a substrate ﬂoating potential of 3.8 V measured during deposition at FS conditions, the substrate bias was varied from + 5 V to − 35 V using a DC voltage source connected to the substrate holder through a resistor (56.2 Ω). The current Ic ﬂowing in the circuit formed by the polarized substrate, the plasma environment and the sputtering chamber (ground) was monitored during the AlN deposition. The scheme of the experimental system with the electrical connections is shown in Fig. 2 (up). As presented in Fig. 2 (down), the timedependent evolution of Ic follows the behavior characteristic of a capacitor charging process, with a transient time during which the arrival of positively charged ions partially compensates the externally applied negative bias at the substrate. After this transient time, Ic saturates to a value Is which increases with negative bias. The variation of substrate bias in the range under study does not have any effect on the growth rate, 60 ± 5 nm/h for all the samples (total growth time = 2 h), or on the RMS surface roughness, 0.6 ±. Substrate bias(V). Ammeter. 8. (b) 8. 6. 4. 2 350. 400. 450. 56.2 Ω Chamber Substrate. Current Intensity, IC (mA). 1.6. FWHM rocking curve (0002) (°). (a) 4.0. 3.2. Effect of the substrate bias. 10. 2.0. 4.5. rms roughness (nm). FWHM rocking curve (0002) (°). The ﬁrst step towards the optimization of AlN deposition consisted in studying the effect of deposition parameters such as RF power (PRF) and substrate temperature (Tsubs) on the layer properties. Taking into account previous results , the sputtering pressure was ﬁxed to 0.47 Pa. A set of AlN layers was deposited at Tsubs = 400 °C with RF power ranging from 100 W to 175 W. For all the samples of this set, the HRXRD 2θ/ωscans show the AlN(0002) diffraction peak with the absence of reﬂections related to other crystal orientations. Fig. 1(a) shows the dependence of the FWHM of the ωscan around the (0002) AlN xray reﬂection peak on PRF. A decrease of this FWHM from 4.26° to 2.18° is observed when increasing PRF from 100 W to 150 W. This amelioration is attributed to the increase of both the Al species energy and the target sputtering rate, the latter resulting in an increase of the growth rate from 40 ± 5 nm/h to 60 ± 5 nm/h within that PRF range. This improvement of crystal quality and growth rate with the RF power is in agreement with results presented by other authors . The effect of sputtering gas rarefaction can be neglected considering the low deposition pressure and atom ﬂux in our experiment (0.47 Pa and 7.8 × 1018 atoms/m2s, respectively) [20,21]. Furthermore, the increase of the energy of the impinging species, and thus their mobility on the growing surface, leads to a decrease of the rootmeansquare (RMS) roughness of the AlN layers from 1.8 nm to 0.3 nm [see Fig. 1(a)]. Further increase of PRF up to 175 W leads to a degradation of the crystalline quality and surface morphology of the layer, with values of FWHM of the AlN(0002) related rocking curve of 3.80° and RMS roughness of 0.6 nm. This degradation of the structural properties can be explained in terms of the growinglayer resputtering by the highly energetic impinging species. Following the obtained results on the effect of PRF, a set of AlN samples were deposited at substrate temperatures ranging from 350 °C to 500 °C, keeping PRF = 150 W. For all the samples of this set, only the peak related to the (0002) reﬂection from AlN was observed in 2θ/ω HRXRD measurements, and the RMS surface roughness measured by AFM on 1 × 1 μm2 surface remains in the range of 0.3–0.6 nm. As it is shown in Fig. 1(b), a minimum FWHM of the rocking curve of 1.91° is. obtained for Tsubs = 450 °C, whereas layers deposited at 350 °C and 500 °C show a FWHM of the (0002) rocking curve as high as 8.77° and 5.78°, respectively. This degradation of the structural quality of the ﬁlms is attributed to the reduction of the mobility of the impinging species at low substrate temperature and to the increase of the desorption rate of physiadsorbed atoms at high substrate temperature . The layer deposited at PRF = 150 W and Tsubs = 450 °C shows a c-lattice parameter of 4.970 Å, which corresponds to a tensile strain of εzz = 0.24%, assuming a relaxed AlN lattice parameter c0 = 4.982 Å . The sample presents a layer thickness of ~115 nm and a grain size of ~40 nm.. 4. 0. -35 V -25 V -15 V -5 V +5 V. -4. 500. Substrate temperature (°C). Fig. 1. (a) FWHM of the rocking curve of the AlN(0002) xray reﬂection and RMS surface roughness of a 1 × 1 μm2 scanned area as a function of the RF power for AlN layers deposited on c-sapphire at a sputtering pressure of 0.47 Pa and Tsubs = 400 °C. The RMS roughness of the sapphire substrate is 0.2 nm. (b) FWHM of the rocking curve of the AlN(0002) xray reﬂection as a function of substrate temperature for AlN layers deposited on c-sapphire at a sputtering pressure of 0.47 Pa and PRF = 150 °C.. Al shutter closed. Al shutter opened. 6. IS (mA). 150. 4 2 0. 0. -20. Substrate Bias (V). 0. 40. 80. -40. 120. Deposition time (min) Fig. 2. (Up) Experimental setup used for the process of biasing the substrate during depositions. (Down) Realtime evolution of the current Ic during deposition for different values of substrate bias. Inset: Saturation intensity, Is, as a function of the substrate bias..
(3) L. Monteagudo-Lerma et al. / Thin Solid Films 545 (2013) 149–153. 2.0. F.S.. 1.6. F.S.. 40. 1.2 0. -20. -40. Substrate bias (V). +5V. Al2O3(0006). -5V -15V -25V. 32. 34. 36. 38 2θ (°). 3.3. Two-step deposition method A two-step deposition method was studied in biased samples to prevent the lattice disorder observed by HRXRD measurements. This twostep method consists ﬁrst of the nucleation of an AlN thin layer (buffer layer) under unbiased substrate conditions, followed by the deposition of negatively biased AlN at −15 V. The buffer thickness is one of the most important parameters of this twostep growth process. It must be optimized to prevent the interface degradation while keeping it as thin as possible, to proﬁt from the structural improvement under negative bias. Fig. 4 shows the HRXRD 2θ/ωscan of two-step samples with unbiased buffer layer thickness of ~15 nm and ~30 nm, compared to an unbiased layer and a layer grown at −15 V bias. The use of an unbiased 15nmthick buffer layer does not fully avoid the formation of lattice disorder, noticeable through a weak and broad peak at 2θ ~ 35°. This can be understood by the fact that the grain size obtained in thick AlN layers deposited using the same conditions as the buffer layer is ~40 nm, signiﬁcantly larger than the buffer layer thickness. Thus a non-homogeneous surface coverage can be expected in a three dimensional growth model . The increase of the buffer layer thickness to 30 nm enables the total suppression of the interface damage (no diffraction peak at 2θ ~ 35°) and leads to a reduction of the FWHM of the AlN(0002) reﬂection peak to 1.63°, to be compared to FWHM = 1.91° for the optimized unbiased layer (see. Biased AlN Two-step d=15 nm Two-step d=30 nm Unbiased AlN. Normalized intensity. F.S.. 50. substrate bias above this value, the estimated ﬁlm density decreases to ~ 2.73 g/cm3 probably due to a change in layer stoichiometry. The observed trend with negative bias is somehow similar to the one described as a function of the RF power (see Section 3.1), i.e., increasing PRF results in a mobility enhancement and thus an improvement of the layer, until a certain threshold (PRF = 175 W) where degradation is associated to the onset of the resputtering process. In summary, within the range of analyzed parameters, the optimized conditions in terms of the FWHM of the (0002) xray reﬂection for AlN growth are PRF = 150 W, Tsubs = 450 °C, and a substrate bias of −15 V. For this substrate bias, the AlN layers show the largest grain size (~55 nm) while keeping low values of FWHM of the x-ray rocking curve (1.35°) and RMS surface roughness (0.6 ± 0.1 nm for a 1 × 1 μm2 scan). However, negative bias is associated to a degradation of the substrate/AlN interface. In the next section, we describe an approach to suppress this damage.. Intensity (arb. units). Intensity (arb. units). AlN(0002). FWHM (°). 2.4. Grain size (nm). 0.1 nm for 1 × 1 μm2 scanning surface. However, differences in the structural quality are observed by HRXRD measurements. Fig. 3 displays the 2θ/ω xray scans for the set of samples deposited under various substrate bias. The diffractograms show the (0002) AlN peak together with a broad reﬂection at 2θ ~35° for negative bias between −5 V and −25 V. This latter reﬂection is attributed to lattice disorder at the AlN/sapphire interface originated by the highly accelerated positive ions (Al+, N+, N+ 2 ), impinging the substrate at the initial stages of the deposition process, during the charging transient observed in Fig. 2. In order to verify that the reﬂection at 2θ ~ 35° is originated by interface damage, we synthesized a sample consisting of a thin (~30nmthick) AlN layer deposited at −15 V bias followed by unbiased AlN with a nominal thickness of 240 nm. Indeed, HRXRD measurements from this sample (not shown) presents the AlN(0002) diffraction peak together with the reﬂection at 2θ ~35°, not observed in any unbiased layer, conﬁrming the presence of lattice disorder at the AlN/substrate interface. Despite the interface damage, the obtained FWHM of the ωscan of the (0002) AlN diffraction peak decreases monotonously when increasing negative bias up to −25 V (see inset of Fig. 3), reaching a best value of 1.25°. The improvement of the structural quality with negative bias can be attributed to an increase of the kinetic energy of the impinging ions, hence increasing the mobility of the adatoms at the growing surface . This is consistent with the observed increase of the grain size, as it is shown in the inset of Fig. 3. A maximum grain size of ~55 nm is achieved for the AlN sample deposited with a substrate bias of −15 V. The AlN ﬁlm deposited at a substrate bias of − 35 V shows the highest value of FWHM of the (0002) reﬂection peak rocking curve in the studied range, namely, 2.23°. The worsening of the structural quality of this sample is attributed to a re-sputtering of the growing surface by the highly accelerated ions . This explanation is supported by the low value of grain size, ~ 35 nm in this sample (see inset of Fig. 3). At the same time, the ﬁlm density estimated by xray reﬂectivity measurements increases from 2.81 g/cm3 to 3.24 g/cm3 with the negative substrate bias from + 5 V to − 15 V. For the sample deposited under − 15 V bias, the ﬁlm density is close to the bulk AlN density (3.27 g/cm3 ). The improved compactness of the layers is attributed to the enhancement of the adatom mobility induced by the increased ion kinetic energy . For. 151. 1.0. 0.5. 0.0. 16. 18. 20. HRXRD ω-scan (°). -35V. 40. 42. 44 33. 34. 35. 36. 37. 38. 39. 40. 41. 2θ (°) Fig. 3. HRXRD 2θ/ωscans of AlN ﬁlms deposited at Tsubs = 450 °C and PRF = 150 W as a function of the substrate bias. The diffractograms are vertically shifted for clarity. Inset: FWHM of the rocking curve of the (0002) reﬂection and grain size as a function of the substrate bias. Best results obtained for AlN deposited under unbiased conditions (ﬂoating substrate, FS) are included as horizontal dashed lines for comparison.. Fig. 4. HRXRD 2θ/ωscans for AlN ﬁlms deposited under various substrate bias conditions: 120nmthick AlN at −15 V, twostep AlN with 15nm and 30nmthick unbiased buffer layer followed by 120nmthick AlN at −15 V, and 120nmthick unbiased AlN. The diffractograms are vertically shifted for clarity..
(4) 152. L. Monteagudo-Lerma et al. / Thin Solid Films 545 (2013) 149–153. (a). (b). (c) 5.50 nm. 0 nm Fig. 5. AFM images of 120nmthick AlN deposited on sapphire (a) at ﬂoating substrate conditions; (b) at −15 V of reverse bias; and (c) at −15 V biased substrate conditions on 30nmthick unbiased AlN buffer layer. The RMS surface roughness of the layers is 0.6, 0.7 nm and 0.4 nm, respectively.. inset of Fig. 4). The grain size of the 30-nm/120-nm two-step AlN layer is ~40 nm and the RMS surface roughness is 0.4 nm, measured in a 1 × 1 μm2 area. This RMS surface roughness value is lower than the values obtained for both the optimized unbiased and biased AlN layers (see AFM images in Fig. 5). 4. Conclusions The inﬂuence of deposition conditions such as RF power, substrate temperature and substrate bias on the morphological and structural properties of cAlN ﬁlms deposited on c-sapphire in pure nitrogen atmosphere by RF reactive sputtering was analyzed. The kinetic energy of impinging ions and thus their mobility at the growing surface is controlled through both the RF power and the substrate bias. The crystalline quality of the layers in terms of grain size and FWHM of the rocking curve is improved when increasing the RF power to an optimal value, established in 150 W for the employed deposition system. Beyond this threshold, further increase of the RF power becomes deleterious for the layer structural properties due to the onset of the resputtering process. The increase of the RF power is accompanied by an enhancement of the growth rate linked to the higher Al sputtering rate. The use of negative bias to increase the kinetic energy of the plasma species during the deposition allows further improvement of the structural quality. Best results are obtained with bias values between −15 V and −25 V, being this range valid for our system conﬁguration and the substrateholder geometry used in this work. The growth rate does not change with the substrate bias since it increases the kinetic energy of the impinging ions but does not affect to the plasma density, so that the amount of available ions for the deposition remains constant. The. improvement of the crystalline quality of the layers under negative substrate bias is accompanied by a degradation of the interface between the AlN layer and the sapphire substrate. This degradation can be avoided by the use of a twostep deposition method consisting of the deposition of an unbiased AlN buffer layer (at least 30 nm thick) prior to the negatively biased (−15 V) AlN layer. The optimized AlN ﬁlm shows a FWHM of the (0002) reﬂection peak of 1.63°, grain size ~40 nm and smooth surface morphology with an RMS surface roughness of 0.4 nm. Acknowledgements Partial ﬁnancial support was provided by the Spanish Government Project, TEC201237958C0201, and by Comunidad de Madrid Project by No. S2009/ESP1781. Xray diffraction measurements were carried out at the Xray Diffraction Techniques Laboratory at the ICMMCSIC.. References  B. Gil, Group III Nitride Semiconductor Compounds, Physics and Applications, Clarendon Press, Oxford, 1998.  Y. Taniyasu, M. Kasu, T. Makimoto, Nature 441 (2006) 325.  Y. Taniyasu, M. Kasu, Appl. Phys. Lett. 99 (2011) 251112.  M.B. Assouar, M. El Hakiki, O. Elmazria, P. Alnot, C. Tiusan, Diamond Relat. Mater. 13 (2004) 1111.  C. Giordano, I. Ingrosso, M.T. Todaro, G. Maruccio, S. De Guido, R. Cingolani, A. Passaseo, M. De Vittorio, Microelectron. Eng. 86 (2009) 1204.  W. Luo, X. Wang, L. Guo, H. Xiao, C. Wang, J. Ran, J. Li, J. Li, Microelectron. J. 39 (2008) 1710.  J.H. Yang, S.M. Kang, D.V. Dinh, D.H. Yoon, Thin Solid Films 517 (2009) 5057.  C. Yen, W. Lai, Y. Yang, C. Wang, T. Ko, S. Hon, S. Chang, IEEE Photon. Technol. Lett. 24 (2012) 294..
(5) L. Monteagudo-Lerma et al. / Thin Solid Films 545 (2013) 149–153  A.V. Lobanova, E.V. Yakovlev, R.A. Talalaev, S.B. Thapa, F. Scholz, J. Cryst. Growth 310 (2008) 4935.  Y. Taniyasu, M. Kasu, T. Makimoto, J. Cryst. Growth 298 (2007) 315.  D.S. Kamber, Y. Wu, B.A. Haskell, S. Newman, S.P. DenBaars, J.S. Speck, S. Nakamura, J. Cryst. Growth 297 (2006) 321.  S. Karmann, H.P.D. Schenk, U. Kaiser, A. Fissel, Wo. Richter, Mater. Sci. Eng. B50 (1997) 228.  G. Koblmüller, R. Averbeck, L. Geelhaar, H. Riechert, W. Hösler, P. Pongratz, J. Appl. Phys. 93 (2003) 9591.  Y. Huttel, H. Gomez, A. Cebollada, G. Armelles, M.I. Alonso, J. Cryst. Growth 242 (2002) 116.  Q.X. Guo, T. Tanaka, M. Nishio, H. Ogawa, Vacuum 80 (2006) 716.  S. Valdueza-Felip, F.B. Naranjo, M. González-Herráez, L. Lahourcade, E. Monroy, S. Fernández, J. Cryst. Growth 312 (2010) 2689.. 153.  A.L. Patterson, Phys. Rev. Am. Phys. Soc. 56 (1939) 978.  I. Horcas, R. Fernandez, J.M. Gomez-Rodriguez, J. Colchero, J. Gomez-Herrero, A.M. Baro, Rev. Sci. Instrum. 78 (2007) 013705.  Z. Vashaei, T. Aikawa, M. Ohtsuka, H. Kobatake, H. Fukuyama, S. Ikeda, K. Takada, J. Cryst. Growth 311 (2009) 459.  S.D. Ekpe, L.W. Bezuidenhout, S.K. Dew, Thin Solid Films 474 (2005) 330.  A. Palmero, H. Rudolph, F.H.P.M. Habraken, Thin Solid Films 515 (2006) 631.  M.E. Levinshtein, S.L. Rumyantsev, M.S. Shur, Properties of Advanced Semiconductor Materials: GaN, AlN, InN, BN, SiC, SiGe, Wiley, New York, 2001.  M. Clement, E. Iborra, J. Sangrador, A. Sanz-Hervás, L. Vergara, M. Aguilar, J. Appl. Phys. 94 (2003) 1495.  H. Seo, I. Petrov, K. Kim, J. Electron. Mater. 39 (2010) 1146.  T.P. Drüsedau, J. Bläsing, Thin Solid Films 27 (2000) 377.  T.J. Kistenmacher, S.A. Ecelberger, W.A. Bryden, J. Appl. Phys. 74 (1993) 1684..